- 325 Views
- Uploaded on
- Presentation posted in: General

CHAPTER 3: CRYSTAL STRUCTURES X-Ray Diffraction (XRD)

Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.

- - - - - - - - - - - - - - - - - - - - - - - - - - E N D - - - - - - - - - - - - - - - - - - - - - - - - - -

ISSUES TO ADDRESS...

- • Historical retrospective
- Henry Bragg Equation
- XRD-analysis
- How to read XRD patterns?
- Exclusions
- What questions can be answered by XRD method?

- Sir William Henry Bragg:
- William Henry and William Lawrence Bragg
- (father and son) found a simple interpretation
- of von Laue’s experiment.
- They assume that each crystal plane reflects radiation as a mirror and analyze this situation for cases of constructive and destructive interference.

Bragg’s law

Noble prize 1915!

Conditions for reflection:

The most important thing in science is not so much to obtain new facts as to discover new ways of thinking about them.

θ

θ

dhkl

θ

x

Path difference Δ= 2x => phase shift

Constructive interference if Δ=nλ

This gives the criterion for constructive interference:

Bragg’s law tells you at which angle θB to expect maximum diffracted intensity for a particular family of crystal planes.

For large crystals, all other angles give zero intensity.

Detector

- The incident angle, w, is defined between the X-ray source and the sample.
- The diffracted angle, 2q, is defined between the incident beam and the detector angle.
- The incident angle w is always ½ of the detector angle 2q .
- In a q:2q instrument (e.g. Rigaku RU300), the tube is fixed, the sample rotates at q°/min and the detector rotates at 2q°/min.
- In a q:q instrument (e.g. PANalytical X’Pert Pro), the sample is fixed and the tube rotates at a rate -q°/min and the detector rotates at a rate of q°/min.

X-ray tube

w

q

2q

2q

The (110) planes would diffract at 29.3 °2q; however, they are not properly aligned to produce a diffraction peak (the perpendicular to those planes does not bisect the incident and diffracted beams). Only background is observed.

The (200) planes are parallel to the (100) planes. Therefore, they also diffract for this crystal. Since d200 is ½ d100, they appear at 42 °2q.

At 20.6 °2q, Bragg’s law fulfilled for the (100) planes, producing a diffraction peak.

2q

2q

2q

- For every set of planes, there will be a small percentage of crystallites that are properly oriented to diffract (the plane perpendicular bisects the incident and diffracted beams).
- Basic assumptions of powder diffraction are that for every set of planes there is an equal number of crystallites that will diffract and that there is a statistically relevant number of crystallites, not just one or two.

- Each peak represents the solution to Bragg’s law for known radiation wavelength (l = 0.154nm)
- The unique relationship between such patterns and crystal structures provide a powerful tool for identification of the phase composition of powders and polycrystalline materials.

The following simple table giving the integer values of FBR for the different types of centering translations. Keep in mind that these are valid for any crystal system.

Summary